On October 23rd, 2014, we updated our
By continuing to use LinkedIn’s SlideShare service, you agree to the revised terms, so please take a few minutes to review them.
AMALGAMATION: TREATING GOLD ORES« on: January 08, 2011, 02:11:58 AM »AMALGAMATION: TREATING GOLD ORESBY AMALGAMATIONIntroductionThe variations of the amalgamation process are as diverse as arethe ores that are treated or the metallurgists who treat them.In this, I will try to cover a little of the history, the hazards, and thetheory of amalgamation. I will then try to show how this experienceand theory can be applied in a practical way to the extraction ofgold from its ores by describing examples of a couple of ancient butstill viable devices. No attempt will be made to give you a cookbooktype method since each ore will demand slightly different details.What I hope to do is provide a basic starting point that can beadjusted as necessary.Historic BackgroundAmalgamation is one of the oldest methods of extracting gold fromits ores. According to Herbert Hoover, in a footnote to histranslation of Georgius Agricolas De Re Metallica, the amalgamationof gold possibly dates from Roman times. The extraction of silver byamalgamation is generally attributed to the Spanish in LatinAmerica in the late sixteenth century even though Biringucciodescribes the fundamental principals of the "patio process" about ahalf a century earlier.The amalgamation of gold ores as described by Agricola in De ReMetallica, which was published in 1556, is essentially the same asmodern practice. The only changes are in the machinery employedand the sources of power to grind, mix, and separate. The use ofwater wheels and of goats in a squirrel cage to provide power towooden machines are just not too common any more. However,although the chemical and physical processes are more clearlyunderstood by more recent authors, the actual "hands on"instructions are remarkably similar and De Re Metallica can still beused as a reference.SafetyBefore going any further into the subject of amalgamation, I will saya few words about the hazards of working with mercury. Like mostthings in our environment it is safe enough if it is treated with duerespect and reasonable precautions are observed. However, theeffects of mercuric poisoning are cumulative and it can doconsiderable damage if mistreated over a long period of time.Mercury can be absorbed through the skin or inhaled in vapor form.
Gloves should be worn whenever it is handled. Be sure that you arein a well ventilated area if there is any possibility of vapors forming.Avoid breathing any of the vapor at all costs.Theory of AmalgamationThe physical and/or chemical characteristics that makeamalgamation work are not clearly understood to this day.However, it is known that if clean mercury is brought into contactwith clean gold, the gold is wetted and "drawn into" the mercury.This results in a solution of gold in mercury or an alloy of gold andmercury called amalgam. After the mercury has gathered in thegold it can be removed by dissolving it in nitric acid or by driving itoff as a vapor by heat. The gold will remain behind.The mill operators problem is to get the gold and the mercury intointimate contact with each other. To do this he must: (1) liberatethe gold particles from the gangue; (2) remove any coating whichmay be covering the gold; (3) keep the mercury clean and bright;and (4) bring the gold and mercury into intimate contact. Then hemust allow the amalgam to coalesce, separate it from the pulp, andextract the gold.Amalgamation generally works best on relatively coarse gold thatcan be liberated from the gangue and abraded clean without toomuch difficulty. Since mercury will not penetrate into minutecrevasses or pores, the ore must be ground fine enough to exposethe gold at the surface. If the gold is very fine, cyanidation is moreeffective and, in practice, a combination of amalgamation andcyanidation is usually employed. Gravity and flotation are alsofrequently used in conjunction with amalgamation.Some of the things that tend to frustrate the millmans attempt toget the mercury and gold together are:1. The existence of surface coatings or encasement of the gold inthe gangue. Fine grinding and abrasion will usually solve thisproblem.2. The presence of oil, grease, clay or iron and base metal sulfidesmay result in sickening or flouring of the mercury. Grinding in limeor some other alkali will usually prevent this occurrence.3. The presence of carbon as graphite also sickens the mercury. Insome instances it can be removed by flotation prior toamalgamation.4. The presence of sulfides of arsenic, antimony or bismuth willcause flouring and sickening of the mercury. This usually makes therecovery of gold by amalgamation impractical.There is some confusion about the meaning of the words flouringand sickening of the mercury. If the mercury will not wet or take upthe gold or coalesce into larger globules it is said to be sick.
Sickening is most likely caused by impurities in or on the surface ofthe mercury. The most common impurities are oil, grease, clay,manganese and iron sulfates, and base metal and iron sulfides.Flouring in the strict sense is the division of the mercury intoextremely small globules. This gives it a white flour-likeappearance. This is not bad in itself but the mercury seems to bemore susceptible to sickening while in the finely divided state.Therefore, it does not coalesce but stays in a floured condition andis lost to tails. Any gold that it took up before becoming sickened isalso lost to tails.MechanismsThe traditional use of amalgamation involved the stamp mill andamalgamation plates. A variation using agitation tubs foramalgamation was described in some detail in De Re Metallica.Today, with the exception of a few traditionalists, the stamp millhas been replaced by the ball mill for this purpose. The mercury isfed into the ball mill with the ore and is then passed over preparedplates.The plates, which should be of pure annealed copper, preferably atleast 1/8 inch think to prevent buckling, must be scoured with sandand lye to remove any coating or oxidation. The resulting brightmetallic copper is then rinsed with clean water and washed with a 2to 3% solution of cyanide if available. Next a mixture of salammoniac and fine sand in equal proportions containing mercury isscrubbed onto the plate and as much mercury as the plate willadsorb is added. After coating the plate should be washed againwith clean water and rinsed with the cyanide solution. Keeping themercury clean will be a problem until the plate builds up a goodgold amalgam coating. To alleviate this problem the plates can besilvered by applying silver amalgam to the prepared plate.The size of plate required will vary with the character of the ore andthe size of the gold particles. If amalgamation is used exclusivelythey should be in the range of 10 to 12 square feet per ton of oreper day. If used in conjunction with cyanidation the area can bereduced to about 1.5 to 4.5 square feet. They should be placed at aslope of 1 1/4 to 2 1/2 inches per foot. The slope should beadjustable to correct for inconsistencies in the ore.Once the plates are loaded, as indicated by the hardening of theamalgam, mercury is sprinkled on the surface to soften it and it isthen scraped with a hard wood or rubber scraper. After theamalgam has been scraped off, mercury is once more added to thesurface and the plate is returned to service.A more practical device for the small miner, and particularly theplacer miner, is the barrel amalgamator. This is simply a horizontal
rotating cylinder in which the slurry of finely ground ore andmercury are placed. The rotation brings the mercury into contactwith the particles of gold. All the problems associated with flouringand sickening of the mercury must be guarded against as with plateamalgamation. This is nearly always a batch operation. A good ruleof thumb is to use about 5 times the amount of mercury as there isgold in the batch. The addition of 3 to 4 pounds of caustic soda perton of ore will help keep both the gold and the mercury clean. Ifnecessary several rocks may be added to the batch to increase theagitation and the abrasion. A cement mixer with the lifts removedmakes an ideal vessel for a small scale operation.For testing or for extremely small scale purposes a copper pan canbe silvered and used in the same manner as the copperamalgamation plate.There is other equipment available for the amalgamation of gold butthey are variations of the two basic types (1) passing the goldbearing slurry over silvered copper plates or (2) adding mercury tothe gold bearing slurry and then retrieving the resulting amalgam.Forgive me but I must bring up my favorite subject; the one thingthat is most often ignored! Everything that goes into the processmust be weighed, sampled, and assayed. Everything that comes outof the process must be weighed, sampled, and assayed. Otherwisethe millman will be operating in ignorance and will have no chanceat all of improving his process or technique.Gold RecoveryAfter the gold has been taken up by the mercury the amalgam mustbe collected. The gold on the plates is scraped off as previouslydescribed. That still in the slurry must be brought together intolarger globules and separated from the slurry. Gravity separation isusually employed. Sluices, jigs, tables, wheels, pans or any othergravity device can be used.The excess mercury can be removed by squeezing it though dampchamois or canvas leaving a hard lump of amalgam. The remainingmercury can then be removed by retorting or by dissolving it indilute nitric acid.Because mercury vaporizes at a much lower temperature than goldit can be driven off by heat leaving the gold behind. In the retortthe mercury vapors are captured and condensed so that themercury can be reused. When using a retort the temperature shouldbe increased gradually until the mercury begins to flow into thereceiver, then backed off slightly and maintained until distillationceases and then increased to a dull red finish. If heated too rapidlythe amalgam may splatter and clog the outlet which could result inthe explosion of the retort.
If a retort is not available, the mercury and silver can be removedby placing the amalgam in hot dilute nitric acid. One part acid tothree parts water is the proportion that works best. The mercuryand silver are dissolved leaving the gold. This solution can then beused to “silver” copper plates or pans or, if economics andconvenience so dictate, it can be discarded.SummaryTo summarize, I want to once more stress the importance of theproper care in the handling and use of mercury. The wearing ofgloves and the adequate ventilation of all work areas are simpleprecautions that can prevent serious health problems.I also want to caution you. Dont get lost in the details andmechanics of the process and forget the fundamentals. Always keepin mind the fact that the whole process depends upon getting clean,bright mercury into contact with clean gold. Anything that promotesthis simple concept is good and anything that restricts it is bad.I sincerely hope that this talk has given you enough informationabout amalgamation to make you want to learn enough to make itwork for you.